#------------------------------------------------------------------------------
#$Date: 2016-03-24 01:35:18 +0200 (Thu, 24 Mar 2016) $
#$Revision: 179537 $
#$URL: svn://www.crystallography.net/cod/cif/4/50/06/4500668.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4500668
loop_
_publ_author_name
'Chen, Lijuan'
'Shi, Dongying'
'Zhao, Junwei'
'Wang, Yulong'
'Ma, Pengtao'
'Wang, Jingping'
'Niu, Jingyang'
_publ_section_title
;
 Three Transition-Metal Substituted Polyoxotungstates Containing Keggin
 Fragments: From Trimer to One-Dimensional Chain to Two-Dimensional Sheet
;
_journal_issue                   5
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              1913
_journal_paper_doi               10.1021/cg200077r
_journal_volume                  11
_journal_year                    2011
_chemical_formula_sum            'H72 K18 Mn9 O156 Si4 W34'
_chemical_formula_weight         10130.10
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   NONE
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                91.844(15)
_cell_angle_beta                 107.857(15)
_cell_angle_gamma                108.924(15)
_cell_formula_units_Z            1
_cell_length_a                   12.722(11)
_cell_length_b                   17.742(16)
_cell_length_c                   20.620(19)
_cell_measurement_reflns_used    2361
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      25.23
_cell_measurement_theta_min      2.27
_cell_volume                     4146(6)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_detector_area_resol_mean NONE
_diffrn_measured_fraction_theta_full 0.989
_diffrn_measured_fraction_theta_max 0.989
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1306
_diffrn_reflns_av_sigmaI/netI    0.2407
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_limit_l_min       -24
_diffrn_reflns_number            20764
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.75
_diffrn_standards_decay_%        NONE
_diffrn_standards_interval_count NONE
_diffrn_standards_interval_time  NONE
_diffrn_standards_number         NONE
_exptl_absorpt_coefficient_mu    24.722
_exptl_absorpt_correction_T_max  0.2765
_exptl_absorpt_correction_T_min  0.1293
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    4.058
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             4459
_exptl_crystal_size_max          0.14
_exptl_crystal_size_mid          0.09
_exptl_crystal_size_min          0.07
_refine_diff_density_max         4.616
_refine_diff_density_min         -5.428
_refine_diff_density_rms         0.671
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.018
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     933
_refine_ls_number_reflns         14455
_refine_ls_number_restraints     216
_refine_ls_restrained_S_all      1.013
_refine_ls_R_factor_all          0.2012
_refine_ls_R_factor_gt           0.1062
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1602P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2548
_refine_ls_wR_factor_ref         0.3116
_reflns_number_gt                7295
_reflns_number_total             14455
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg200077r_si_002.cif
_cod_data_source_block           2
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.1 from
2010-06-29.

'_exptl_absorpt_correction_type' value 'MULTI-SCAN'
changed to 'multi-scan' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from
2010-06-29.

'_refine_ls_hydrogen_treatment' value 'CONSTR' changed
to 'constr' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_cell_volume        4145(6)
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               4500668
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.89656(18) 0.80307(11) -0.32382(9) 0.0448(6) Uani 1 1 d . . .
W2 W 0.73231(15) 0.90895(10) -0.30315(8) 0.0351(5) Uani 1 1 d . . .
W3 W 0.91344(16) 0.97427(10) -0.39250(8) 0.0352(5) Uani 1 1 d . . .
W4 W 1.23221(16) 1.05085(11) -0.30924(8) 0.0362(5) Uani 1 1 d . . .
W5 W 1.35425(15) 1.06098(11) -0.14069(8) 0.0357(5) Uani 1 1 d . . .
W6 W 1.22231(17) 0.88169(11) -0.23641(9) 0.0403(5) Uani 1 1 d . . .
W7 W 1.16079(15) 0.90647(10) -0.07253(8) 0.0324(5) Uani 1 1 d . . .
W8 W 0.87618(15) 0.84139(10) -0.14477(8) 0.0322(5) Uani 1 1 d . . .
W9 W 1.14457(19) 1.31907(10) -0.06647(9) 0.0471(6) Uani 1 1 d . . .
W10 W 0.85316(17) 1.24552(11) -0.14365(8) 0.0369(5) Uani 1 1 d . . .
W11 W 0.9978(2) 1.44466(12) -0.11910(10) 0.0623(8) Uani 1 1 d . A .
W12 W 0.7272(2) 1.24243(17) -0.32881(13) 0.0336(8) Uani 0.624(2) 1 d P A 1
W13 W 0.9052(3) 1.32357(18) -0.41757(13) 0.0394(8) Uani 0.624(2) 1 d P A 1
W14 W 0.8645(3) 1.44383(17) -0.30684(14) 0.0391(8) Uani 0.624(2) 1 d P A 1
W15 W 1.2694(3) 1.48904(17) -0.14187(16) 0.0421(8) Uani 0.624(2) 1 d P A 1
W16 W 1.3211(3) 1.37090(19) -0.25160(16) 0.0446(9) Uani 0.624(2) 1 d P A 1
W17 W 1.1638(3) 1.49089(19) -0.30982(16) 0.0469(9) Uani 0.624(2) 1 d P A 1
W18 W 1.3570(4) 1.3914(3) -0.1724(3) 0.0382(13) Uani 0.376(2) 1 d P A 2
W19 W 1.2219(10) 1.5290(6) -0.2260(5) 0.056(3) Uani 0.376(2) 1 d P A 2
W20 W 1.2437(5) 1.3966(3) -0.3396(3) 0.0429(14) Uani 0.376(2) 1 d P A 2
W21 W 0.8079(5) 1.2324(3) -0.4000(3) 0.0528(17) Uani 0.376(2) 1 d P A 2
W22 W 0.9660(5) 1.4314(3) -0.3771(3) 0.0505(16) Uani 0.376(2) 1 d P A 2
W23 W 0.7924(5) 1.3663(4) -0.2834(3) 0.0554(19) Uani 0.376(2) 1 d P A 2
Si1 Si 1.0420(9) 0.9881(6) -0.2152(5) 0.023(3) Uani 1 1 d . A .
Si2 Si 1.0373(11) 1.3160(6) -0.2430(5) 0.031(3) Uani 1 1 d . A .
Mn1 Mn 0.6496(6) 1.2033(4) -0.0381(3) 0.0380(17) Uani 1 1 d . . .
Mn2 Mn 0.9021(5) 1.1162(4) -0.2649(3) 0.0283(15) Uani 1 1 d . A .
Mn3 Mn 1.1800(6) 1.1840(4) -0.1919(3) 0.0347(16) Uani 1 1 d . A .
Mn4 Mn 1.0721(6) 1.1870(4) -0.3525(3) 0.0385(17) Uani 1 1 d . A .
Mn5 Mn 1.0000 1.0000 0.0000 0.032(2) Uani 1 2 d S . .
K1 K 0.6765(18) 0.6366(10) -0.1253(7) 0.120(7) Uani 1 1 d . . .
K2 K 0.9829(16) 0.6693(8) -0.0620(7) 0.093(5) Uani 1 1 d . . .
K3 K 0.7461(11) 1.0220(9) -0.1330(6) 0.077(4) Uani 1 1 d . . .
O1 O 0.858(3) 0.7057(16) -0.3625(16) 0.053(9) Uani 1 1 d . . .
O2 O 0.746(2) 0.8050(15) -0.3324(13) 0.030(7) Uani 1 1 d . . .
O3 O 0.898(2) 0.8576(15) -0.3995(12) 0.029(6) Uani 1 1 d U . .
O4 O 0.913(2) 0.7920(15) -0.2282(13) 0.031(6) Uani 1 1 d U . .
O5 O 1.067(3) 0.8343(16) -0.2974(14) 0.042(7) Uani 1 1 d U . .
O6 O 0.934(2) 0.9392(15) -0.2828(13) 0.030(6) Uani 1 1 d U . .
O7 O 0.585(3) 0.8732(18) -0.3246(15) 0.048(8) Uani 1 1 d U . .
O8 O 0.757(3) 0.9329(17) -0.3879(14) 0.042(7) Uani 1 1 d U . .
O9 O 0.767(2) 1.0112(13) -0.2670(13) 0.027(6) Uani 1 1 d . . .
O10 O 0.778(2) 0.8791(16) -0.2107(14) 0.039(7) Uani 1 1 d U . .
O11 O 0.881(3) 0.9800(17) -0.4802(14) 0.045(7) Uani 1 1 d U . .
O12 O 1.078(2) 0.9941(15) -0.3718(13) 0.032(6) Uani 1 1 d U . .
O13 O 0.935(3) 1.0737(16) -0.3555(13) 0.037(8) Uani 1 1 d . . .
O14 O 1.304(2) 1.0830(18) -0.3638(17) 0.051(9) Uani 1 1 d . . .
O15 O 1.195(3) 1.1360(16) -0.2908(13) 0.046(9) Uani 1 1 d . . .
O16 O 1.363(2) 1.0842(15) -0.2282(13) 0.030(6) Uani 1 1 d U . .
O17 O 1.249(3) 0.9434(18) -0.3057(13) 0.046(8) Uani 1 1 d . . .
O18 O 1.168(2) 0.9975(13) -0.2235(12) 0.024(6) Uani 1 1 d U . .
O19 O 1.500(2) 1.1011(16) -0.0859(14) 0.040(7) Uani 1 1 d U . .
O20 O 1.356(2) 0.9540(15) -0.1748(14) 0.039(7) Uani 1 1 d U . .
O21 O 1.304(3) 1.1389(16) -0.1263(14) 0.044(8) Uani 1 1 d . . .
O22 O 1.276(2) 1.0009(16) -0.0845(13) 0.035(7) Uani 1 1 d U . .
O23 O 1.267(3) 0.8026(19) -0.2531(18) 0.068(11) Uani 1 1 d . . .
O24 O 1.163(3) 0.8553(16) -0.1677(15) 0.044(8) Uani 1 1 d . . .
O25 O 1.248(3) 0.8608(19) -0.0236(15) 0.050(9) Uani 1 1 d . . .
O26 O 1.007(2) 0.8186(17) -0.0936(12) 0.034(7) Uani 1 1 d . . .
O27 O 1.136(2) 0.9632(17) -0.0105(14) 0.037(7) Uani 1 1 d . . .
O28 O 1.026(3) 0.9400(18) -0.1518(12) 0.044(9) Uani 1 1 d . . .
O29 O 0.778(3) 0.750(2) -0.1404(18) 0.054(9) Uani 1 1 d . . .
O30 O 0.878(3) 0.9024(17) -0.0737(15) 0.045(8) Uani 1 1 d . . .
O31 O 1.222(3) 1.3260(19) 0.0198(17) 0.059(9) Uani 1 1 d U . .
O32 O 1.093(3) 1.4153(18) -0.0504(17) 0.059(9) Uani 1 1 d U . .
O33 O 1.255(3) 1.3921(17) -0.0962(14) 0.044(7) Uani 1 1 d U . .
O34 O 0.991(3) 1.2627(15) -0.0624(13) 0.039(8) Uani 1 1 d . . .
O35 O 1.164(2) 1.2370(16) -0.1042(14) 0.038(7) Uani 1 1 d U . .
O36 O 1.013(3) 1.3254(17) -0.1697(14) 0.060(10) Uani 1 1 d . . .
O37 O 0.748(3) 1.2031(18) -0.1126(14) 0.047(9) Uani 1 1 d . . .
O38 O 0.770(3) 1.268(2) -0.2295(17) 0.063(9) Uani 1 1 d U . .
O39 O 0.875(3) 1.3590(14) -0.1124(12) 0.033(6) Uani 1 1 d U . .
O40 O 0.871(2) 1.1593(13) -0.1788(12) 0.023(6) Uani 1 1 d U . .
O41 O 0.982(3) 1.525(2) -0.0782(17) 0.065(10) Uani 1 1 d U . .
O42 O 1.120(3) 1.4949(18) -0.1427(16) 0.052(8) Uani 1 1 d U . .
O43 O 0.908(3) 1.4443(18) -0.2102(12) 0.039(8) Uani 1 1 d . . .
O44 O 1.313(3) 1.2894(19) -0.1957(17) 0.058(10) Uani 1 1 d . . .
O45 O 0.742(4) 1.355(2) -0.3160(19) 0.058 Uiso 1 1 d . . .
O46 O 0.757(3) 1.275(2) -0.4116(18) 0.064 Uiso 1 1 d . . .
O47 O 0.781(3) 1.1596(19) -0.3284(17) 0.063(11) Uani 1 1 d . . .
O48 O 0.927(3) 1.3280(16) -0.3031(13) 0.050(10) Uani 1 1 d . . .
O49 O 0.874(4) 1.331(3) -0.505(3) 0.108(16) Uani 1 1 d U . .
O50 O 0.849(3) 1.4097(18) -0.3906(15) 0.050 Uiso 1 1 d . . .
O51 O 0.954(3) 1.236(2) -0.4100(16) 0.057(9) Uani 1 1 d U . .
O52 O 1.071(3) 1.405(2) -0.3818(18) 0.066(10) Uani 1 1 d U . .
O53 O 0.818(3) 1.5234(19) -0.3152(16) 0.055 Uiso 1 1 d . . .
O54 O 1.036(3) 1.4966(18) -0.2899(17) 0.066(11) Uani 1 1 d . . .
O55 O 1.363(3) 1.5694(19) -0.0715(17) 0.059 Uiso 1 1 d . . .
O56 O 1.240(4) 1.519(3) -0.221(2) 0.011(10) Uiso 1 1 d . . .
O57 O 1.381(3) 1.454(2) -0.1707(18) 0.068 Uiso 1 1 d . . .
O58 O 1.159(3) 1.3870(17) -0.2422(14) 0.045(8) Uani 1 1 d U . .
O59 O 1.454(3) 1.388(2) -0.2635(18) 0.066 Uiso 1 1 d . . .
O60 O 1.292(4) 1.453(3) -0.309(2) 0.083(12) Uani 1 1 d U . .
O61 O 1.215(3) 1.2940(17) -0.3401(15) 0.042(7) Uani 1 1 d U . .
O62 O 1.192(3) 1.5682(19) -0.3525(17) 0.059 Uiso 1 1 d . . .
O63 O 0.579(3) 1.199(3) -0.353(2) 0.098(16) Uani 1 1 d . . .
O64 O 1.035(2) 1.0765(13) -0.1999(11) 0.020(5) Uani 1 1 d U . .
O65 O 1.044(2) 1.2280(14) -0.2584(11) 0.023(6) Uani 1 1 d U . .
O1W O 0.561(4) 1.200(2) 0.038(2) 0.080(12) Uani 1 1 d U . .
O2W O 0.559(3) 1.277(2) -0.1004(19) 0.069(10) Uani 1 1 d U . .
O3W O 0.772(4) 1.320(2) 0.024(2) 0.079 Uiso 1 1 d . . .
O4W O 1.104(3) 1.1514(19) -0.4475(14) 0.050(9) Uani 1 1 d . . .
O5W O 0.993(3) 0.9131(16) 0.0760(14) 0.041(7) Uani 1 1 d U . .
O6W O 1.361(2) 1.2892(14) 0.0890(12) 0.028(6) Uani 1 1 d U . .
O7W O 1.284(2) 1.1645(14) 0.0033(11) 0.020(5) Uani 1 1 d U . .
O8W O 0.894(3) 1.133(2) 0.4447(15) 0.073(12) Uani 1 1 d . . .
O9W O 0.388(3) 1.248(2) -0.3647(17) 0.059(10) Uani 1 1 d . . .
O10W O 1.396(4) 1.075(3) -0.4734(17) 0.085(13) Uani 1 1 d . . .
O11W O 1.248(4) 1.554(2) 0.045(3) 0.13(2) Uani 1 1 d . . .
O12W O 1.071(5) 0.660(3) -0.345(3) 0.14(2) Uiso 1 1 d . . .
O13W O 0.521(7) 1.241(4) -0.231(4) 0.07(2) Uiso 0.50 1 d P . .
O14W O 1.380(9) 0.930(6) -0.385(5) 0.11(3) Uiso 0.50 1 d P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 W1 O3 100.0(13) . .
O1 W1 O2 99.9(14) . .
O3 W1 O2 90.7(12) . .
O1 W1 O4 103.8(13) . .
O3 W1 O4 156.2(10) . .
O2 W1 O4 85.5(11) . .
O1 W1 O5 98.3(14) . .
O3 W1 O5 88.5(12) . .
O2 W1 O5 161.7(10) . .
O4 W1 O5 87.9(12) . .
O1 W1 O6 173.3(12) . .
O3 W1 O6 74.6(10) . .
O2 W1 O6 76.5(9) . .
O4 W1 O6 81.7(10) . .
O5 W1 O6 85.6(10) . .
O7 W2 O9 101.1(13) . .
O7 W2 O8 103.6(13) . .
O9 W2 O8 96.4(12) . .
O7 W2 O10 100.4(13) . .
O9 W2 O10 90.7(12) . .
O8 W2 O10 153.1(12) . .
O7 W2 O2 95.9(12) . .
O9 W2 O2 162.9(10) . .
O8 W2 O2 81.8(11) . .
O10 W2 O2 83.9(11) . .
O7 W2 O6 170.9(12) . .
O9 W2 O6 88.0(10) . .
O8 W2 O6 73.8(11) . .
O10 W2 O6 80.6(11) . .
O2 W2 O6 75.2(9) . .
O7 W2 K3 87.8(11) . .
O9 W2 K3 42.7(9) . .
O8 W2 K3 139.1(8) . .
O10 W2 K3 53.3(8) . .
O2 W2 K3 136.8(8) . .
O6 W2 K3 99.9(6) . .
O11 W3 O13 103.6(12) . .
O11 W3 O12 96.8(13) . .
O13 W3 O12 94.3(12) . .
O11 W3 O8 100.1(13) . .
O13 W3 O8 91.7(12) . .
O12 W3 O8 160.2(12) . .
O11 W3 O3 96.3(11) . .
O13 W3 O3 160.0(11) . .
O12 W3 O3 84.3(11) . .
O8 W3 O3 83.6(11) . .
O11 W3 O6 168.4(11) . .
O13 W3 O6 86.7(10) . .
O12 W3 O6 87.5(10) . .
O8 W3 O6 74.0(10) . .
O3 W3 O6 73.3(9) . .
O14 W4 O15 101.4(14) . .
O14 W4 O16 97.5(13) . .
O15 W4 O16 90.4(12) . .
O14 W4 O12 100.8(13) . .
O15 W4 O12 92.5(13) . .
O16 W4 O12 160.5(12) . .
O14 W4 O17 98.0(14) . .
O15 W4 O17 160.5(13) . .
O16 W4 O17 85.5(10) . .
O12 W4 O17 85.3(11) . .
O14 W4 O18 167.3(12) . .
O15 W4 O18 87.6(11) . .
O16 W4 O18 73.2(10) . .
O12 W4 O18 87.7(10) . .
O17 W4 O18 73.0(10) . .
O19 W5 O21 100.6(12) . .
O19 W5 O22 102.7(12) . .
O21 W5 O22 89.9(14) . .
O19 W5 O16 104.1(13) . .
O21 W5 O16 94.9(12) . .
O22 W5 O16 151.4(11) . .
O19 W5 O20 98.1(12) . .
O21 W5 O20 161.1(12) . .
O22 W5 O20 83.8(12) . .
O16 W5 O20 82.7(11) . .
O19 W5 O18 172.1(11) . .
O21 W5 O18 86.3(10) . .
O22 W5 O18 80.9(10) . .
O16 W5 O18 71.3(10) . .
O20 W5 O18 75.1(9) . .
O23 W6 O24 104.6(14) . .
O23 W6 O20 102.9(15) . .
O24 W6 O20 89.9(13) . .
O23 W6 O5 95.5(14) . .
O24 W6 O5 87.0(13) . .
O20 W6 O5 161.6(11) . .
O23 W6 O17 101.7(15) . .
O24 W6 O17 153.3(12) . .
O20 W6 O17 89.1(12) . .
O5 W6 O17 85.6(13) . .
O23 W6 O18 173.5(14) . .
O24 W6 O18 81.9(10) . .
O20 W6 O18 76.9(10) . .
O5 W6 O18 84.7(9) . .
O17 W6 O18 71.9(11) . .
O25 W7 O27 102.8(14) . .
O25 W7 O22 101.0(13) . .
O27 W7 O22 91.1(12) . .
O25 W7 O26 98.8(13) . .
O27 W7 O26 93.6(12) . .
O22 W7 O26 158.1(11) . .
O25 W7 O24 93.8(13) . .
O27 W7 O24 163.3(11) . .
O22 W7 O24 84.4(11) . .
O26 W7 O24 85.0(11) . .
O25 W7 O28 167.2(13) . .
O27 W7 O28 87.0(11) . .
O22 W7 O28 86.9(11) . .
O26 W7 O28 72.0(12) . .
O24 W7 O28 76.8(9) . .
O25 W7 K3 67.1(11) . 2_775
O27 W7 K3 36.0(9) . 2_775
O22 W7 K3 93.4(8) . 2_775
O26 W7 K3 103.0(8) . 2_775
O24 W7 K3 160.1(7) . 2_775
O28 W7 K3 122.9(7) . 2_775
O25 W7 K2 66.3(11) . .
O27 W7 K2 104.7(10) . .
O22 W7 K2 161.4(8) . .
O26 W7 K2 32.8(8) . .
O24 W7 K2 83.0(8) . .
O28 W7 K2 103.4(9) . .
K3 W7 K2 93.8(3) 2_775 .
O29 W8 O30 100.6(15) . .
O29 W8 O10 100.8(14) . .
O30 W8 O10 94.8(12) . .
O29 W8 O26 93.5(13) . .
O30 W8 O26 93.7(12) . .
O10 W8 O26 161.6(13) . .
O29 W8 O4 92.9(13) . .
O30 W8 O4 166.0(13) . .
O10 W8 O4 86.4(11) . .
O26 W8 O4 81.5(10) . .
O29 W8 O28 166.1(11) . .
O30 W8 O28 88.6(12) . .
O10 W8 O28 88.6(11) . .
O26 W8 O28 75.4(11) . .
O4 W8 O28 77.5(10) . .
O29 W8 K1 4.0(11) . .
O30 W8 K1 100.0(11) . .
O10 W8 K1 104.8(9) . .
O26 W8 K1 89.7(9) . .
O4 W8 K1 93.2(8) . .
O28 W8 K1 163.3(7) . .
O29 W8 K2 58.1(10) . .
O30 W8 K2 104.5(9) . .
O10 W8 K2 153.4(9) . .
O26 W8 K2 36.0(9) . .
O4 W8 K2 79.3(7) . .
O28 W8 K2 109.8(7) . .
K1 W8 K2 54.3(4) . .
O29 W8 K3 111.2(10) . .
O30 W8 K3 47.4(9) . .
O10 W8 K3 47.8(9) . .
O26 W8 K3 135.9(8) . .
O4 W8 K3 130.4(7) . .
O28 W8 K3 82.6(7) . .
K1 W8 K3 113.7(4) . .
K2 W8 K3 150.3(3) . .
O31 W9 O35 102.9(13) . .
O31 W9 O33 102.1(14) . .
O35 W9 O33 92.0(14) . .
O31 W9 O34 97.0(15) . .
O35 W9 O34 97.5(12) . .
O33 W9 O34 156.2(11) . .
O31 W9 O32 93.3(13) . .
O35 W9 O32 163.8(12) . .
O33 W9 O32 84.9(14) . .
O34 W9 O32 79.9(13) . .
O31 W9 O36 164.5(14) . .
O35 W9 O36 90.9(11) . .
O33 W9 O36 84.1(12) . .
O34 W9 O36 74.0(12) . .
O32 W9 O36 73.0(11) . .
O31 W9 K2 58.4(12) . 2_775
O35 W9 K2 130.3(10) . 2_775
O33 W9 K2 134.7(9) . 2_775
O34 W9 K2 48.2(8) . 2_775
O32 W9 K2 58.9(10) . 2_775
O36 W9 K2 107.2(10) . 2_775
O31 W9 K1 7.3(11) . 2_775
O35 W9 K1 109.2(9) . 2_775
O33 W9 K1 97.7(8) . 2_775
O34 W9 K1 99.7(8) . 2_775
O32 W9 K1 87.0(9) . 2_775
O36 W9 K1 159.7(8) . 2_775
K2 W9 K1 57.6(4) 2_775 2_775
O37 W10 O40 101.0(13) . .
O37 W10 O38 102.4(14) . .
O40 W10 O38 95.5(13) . .
O37 W10 O34 100.1(12) . .
O40 W10 O34 91.4(10) . .
O38 W10 O34 154.7(14) . .
O37 W10 O39 96.1(14) . .
O40 W10 O39 162.8(12) . .
O38 W10 O39 82.4(12) . .
O34 W10 O39 83.9(10) . .
O37 W10 O36 168.6(12) . .
O40 W10 O36 88.9(11) . .
O38 W10 O36 82.1(14) . .
O34 W10 O36 73.8(11) . .
O39 W10 O36 73.9(11) . .
O37 W10 K3 57.4(10) . .
O40 W10 K3 44.5(9) . .
O38 W10 K3 111.4(10) . .
O34 W10 K3 90.4(8) . .
O39 W10 K3 151.5(9) . .
O36 W10 K3 131.0(8) . .
O37 W10 K2 78.3(10) . 2_775
O40 W10 K2 119.4(7) . 2_775
O38 W10 K2 144.5(11) . 2_775
O34 W10 K2 32.8(9) . 2_775
O39 W10 K2 62.4(7) . 2_775
O36 W10 K2 91.9(7) . 2_775
K3 W10 K2 98.9(3) . 2_775
O41 W11 O42 100.4(16) . .
O41 W11 O32 102.5(16) . .
O42 W11 O32 88.1(15) . .
O41 W11 O39 102.1(15) . .
O42 W11 O39 157.5(12) . .
O32 W11 O39 87.8(14) . .
O41 W11 O43 100.2(14) . .
O42 W11 O43 85.6(13) . .
O32 W11 O43 157.2(14) . .
O39 W11 O43 89.7(12) . .
O41 W11 O36 175.1(15) . .
O42 W11 O36 83.9(13) . .
O32 W11 O36 75.1(13) . .
O39 W11 O36 73.6(12) . .
O43 W11 O36 82.5(11) . .
O63 W12 O47 105.4(18) . .
O63 W12 O46 105(2) . .
O47 W12 O46 94.5(16) . .
O63 W12 O45 99.5(19) . .
O47 W12 O45 155.1(16) . .
O46 W12 O45 79.6(15) . .
O63 W12 O38 101(2) . .
O47 W12 O38 97.6(14) . .
O46 W12 O38 147.0(14) . .
O45 W12 O38 76.5(15) . .
O63 W12 O48 167.7(18) . .
O47 W12 O48 86.1(13) . .
O46 W12 O48 69.3(12) . .
O45 W12 O48 69.2(13) . .
O38 W12 O48 81.1(13) . .
O49 W13 O46 102(2) . .
O49 W13 O51 102.6(18) . .
O46 W13 O51 98.7(16) . .
O49 W13 O50 98.5(18) . .
O46 W13 O50 71.3(15) . .
O51 W13 O50 158.2(14) . .
O49 W13 O52 98.9(19) . .
O46 W13 O52 152.2(15) . .
O51 W13 O52 93.8(14) . .
O50 W13 O52 88.2(14) . .
O49 W13 O48 169.6(17) . .
O46 W13 O48 72.8(14) . .
O51 W13 O48 87.3(12) . .
O50 W13 O48 71.3(11) . .
O52 W13 O48 83.2(13) . .
O53 W14 O50 104.2(15) . .
O53 W14 O45 109.0(17) . .
O50 W14 O45 85.3(16) . .
O53 W14 O43 101.0(13) . .
O50 W14 O43 154.8(13) . .
O45 W14 O43 88.0(15) . .
O53 W14 O54 101.8(14) . .
O50 W14 O54 87.8(15) . .
O45 W14 O54 149.1(15) . .
O43 W14 O54 85.6(13) . .
O53 W14 O48 176.3(12) . .
O50 W14 O48 72.1(12) . .
O45 W14 O48 70.4(15) . .
O43 W14 O48 82.7(10) . .
O54 W14 O48 78.9(12) . .
O56 W15 O55 114.6(18) . .
O56 W15 O42 86.7(18) . .
O55 W15 O42 97.6(15) . .
O56 W15 O57 83.0(18) . .
O55 W15 O57 103.7(16) . .
O42 W15 O57 158.7(13) . .
O56 W15 O33 142.1(16) . .
O55 W15 O33 102.7(13) . .
O42 W15 O33 95.4(14) . .
O57 W15 O33 81.8(15) . .
O56 W15 O58 61.5(16) . .
O55 W15 O58 174.0(15) . .
O42 W15 O58 86.9(12) . .
O57 W15 O58 71.8(13) . .
O33 W15 O58 80.8(10) . .
O59 W16 O44 103.2(16) . .
O59 W16 O60 90.8(18) . .
O44 W16 O60 166.0(17) . .
O59 W16 O57 96.2(16) . .
O44 W16 O57 91.1(15) . .
O60 W16 O57 87.7(17) . .
O59 W16 O61 98.7(14) . .
O44 W16 O61 94.3(13) . .
O60 W16 O61 83.1(15) . .
O57 W16 O61 162.5(14) . .
O59 W16 O58 162.5(14) . .
O44 W16 O58 92.7(13) . .
O60 W16 O58 73.5(15) . .
O57 W16 O58 75.9(13) . .
O61 W16 O58 87.3(11) . .
O62 W17 O56 111.8(18) . .
O62 W17 O54 101.5(16) . .
O56 W17 O54 85.7(18) . .
O62 W17 O52 102.0(15) . .
O56 W17 O52 145.8(18) . .
O54 W17 O52 93.1(15) . .
O62 W17 O60 100.4(18) . .
O56 W17 O60 84.1(18) . .
O54 W17 O60 158.0(16) . .
O52 W17 O60 84.6(17) . .
O62 W17 O58 170.2(15) . .
O56 W17 O58 62.9(16) . .
O54 W17 O58 86.7(12) . .
O52 W17 O58 82.8(12) . .
O60 W17 O58 71.3(15) . .
O57 W18 O44 166(2) . .
O57 W18 O33 91(2) . .
O44 W18 O33 99.1(15) . .
O57 W18 O58 85(2) . .
O44 W18 O58 89.3(12) . .
O33 W18 O58 73.4(10) . .
O54 W19 O58 78.5(11) . .
O54 W19 O42 77.3(13) . .
O58 W19 O42 77.9(11) . .
O60 W20 O61 143(2) . .
O60 W20 O52 102(3) . .
O61 W20 O52 103.5(14) . .
O46 W21 O51 132(2) . .
O46 W21 O47 118(2) . .
O51 W21 O47 106.6(14) . .
O46 W21 O48 83.7(18) . .
O51 W21 O48 84.7(13) . .
O47 W21 O48 82.8(11) . .
O50 W22 O52 146.4(19) . .
O50 W22 O54 105.5(18) . .
O52 W22 O54 101.0(17) . .
O50 W22 O48 77.1(15) . .
O52 W22 O48 87.8(15) . .
O54 W22 O48 80.1(11) . .
O45 W23 O43 151(3) . .
O45 W23 O38 107(3) . .
O43 W23 O38 97.8(12) . .
O45 W23 O48 106(3) . .
O43 W23 O48 90.5(11) . .
O38 W23 O48 83.5(13) . .
O6 Si1 O28 107.6(16) . .
O6 Si1 O18 111.8(14) . .
O28 Si1 O18 110.0(14) . .
O6 Si1 O64 108.7(12) . .
O28 Si1 O64 108.6(13) . .
O18 Si1 O64 110.1(14) . .
O65 Si2 O58 110.4(16) . .
O65 Si2 O48 110.8(13) . .
O58 Si2 O48 107.5(16) . .
O65 Si2 O36 110.3(15) . .
O58 Si2 O36 111.3(17) . .
O48 Si2 O36 106.4(18) . .
O19 Mn1 O25 95.5(11) 1_455 2_775
O19 Mn1 O1W 81.5(13) 1_455 .
O25 Mn1 O1W 89.1(14) 2_775 .
O19 Mn1 O3W 163.6(14) 1_455 .
O25 Mn1 O3W 91.8(14) 2_775 .
O1W Mn1 O3W 84.0(15) . .
O19 Mn1 O2W 88.7(12) 1_455 .
O25 Mn1 O2W 175.4(14) 2_775 .
O1W Mn1 O2W 93.4(15) . .
O3W Mn1 O2W 84.6(14) . .
O19 Mn1 O37 99.0(12) 1_455 .
O25 Mn1 O37 87.6(11) 2_775 .
O1W Mn1 O37 176.7(13) . .
O3W Mn1 O37 96.0(14) . .
O2W Mn1 O37 90.0(12) . .
O47 Mn2 O9 90.3(13) . .
O47 Mn2 O40 89.7(11) . .
O9 Mn2 O40 84.7(10) . .
O47 Mn2 O64 176.9(13) . .
O9 Mn2 O64 92.8(10) . .
O40 Mn2 O64 91.2(9) . .
O47 Mn2 O65 90.2(12) . .
O9 Mn2 O65 177.7(10) . .
O40 Mn2 O65 93.0(9) . .
O64 Mn2 O65 86.7(9) . .
O47 Mn2 O13 89.5(12) . .
O9 Mn2 O13 96.3(11) . .
O40 Mn2 O13 178.7(10) . .
O64 Mn2 O13 89.6(9) . .
O65 Mn2 O13 86.0(10) . .
O47 Mn2 Mn3 134.8(11) . .
O9 Mn2 Mn3 134.9(7) . .
O40 Mn2 Mn3 93.3(6) . .
O64 Mn2 Mn3 42.2(7) . .
O65 Mn2 Mn3 44.5(6) . .
O13 Mn2 Mn3 86.6(8) . .
O47 Mn2 Mn4 88.1(11) . .
O9 Mn2 Mn4 138.7(7) . .
O40 Mn2 Mn4 136.5(7) . .
O64 Mn2 Mn4 89.2(7) . .
O65 Mn2 Mn4 43.6(6) . .
O13 Mn2 Mn4 42.5(8) . .
Mn3 Mn2 Mn4 59.8(2) . .
O47 Mn2 K3 102.7(11) . .
O9 Mn2 K3 44.5(8) . .
O40 Mn2 K3 43.3(7) . .
O64 Mn2 K3 80.0(7) . .
O65 Mn2 K3 133.2(7) . .
O13 Mn2 K3 137.9(8) . .
Mn3 Mn2 K3 110.1(3) . .
Mn4 Mn2 K3 169.0(3) . .
O44 Mn3 O35 92.1(13) . .
O44 Mn3 O21 92.7(12) . .
O35 Mn3 O21 89.2(10) . .
O44 Mn3 O64 173.6(11) . .
O35 Mn3 O64 91.9(10) . .
O21 Mn3 O64 92.3(10) . .
O44 Mn3 O65 89.7(11) . .
O35 Mn3 O65 89.4(9) . .
O21 Mn3 O65 177.3(12) . .
O64 Mn3 O65 85.4(9) . .
O44 Mn3 O15 84.9(13) . .
O35 Mn3 O15 175.1(10) . .
O21 Mn3 O15 94.9(11) . .
O64 Mn3 O15 90.7(10) . .
O65 Mn3 O15 86.6(9) . .
O44 Mn3 Mn2 132.8(9) . .
O35 Mn3 Mn2 91.4(8) . .
O21 Mn3 Mn2 134.5(9) . .
O64 Mn3 Mn2 42.2(6) . .
O65 Mn3 Mn2 43.2(7) . .
O15 Mn3 Mn2 87.7(9) . .
O44 Mn3 Mn4 83.7(9) . .
O35 Mn3 Mn4 133.2(7) . .
O21 Mn3 Mn4 137.4(8) . .
O64 Mn3 Mn4 89.9(6) . .
O65 Mn3 Mn4 44.2(6) . .
O15 Mn3 Mn4 42.6(7) . .
Mn2 Mn3 Mn4 60.7(2) . .
O51 Mn4 O61 91.7(13) . .
O51 Mn4 O15 179.0(13) . .
O61 Mn4 O15 88.6(12) . .
O51 Mn4 O13 93.6(12) . .
O61 Mn4 O13 174.1(11) . .
O15 Mn4 O13 86.0(11) . .
O51 Mn4 O65 89.3(11) . .
O61 Mn4 O65 91.9(11) . .
O15 Mn4 O65 89.7(9) . .
O13 Mn4 O65 85.6(10) . .
O51 Mn4 O4W 89.9(12) . .
O61 Mn4 O4W 85.8(12) . .
O15 Mn4 O4W 91.1(10) . .
O13 Mn4 O4W 96.8(11) . .
O65 Mn4 O4W 177.5(11) . .
O51 Mn4 Mn3 133.6(10) . .
O61 Mn4 Mn3 87.7(8) . .
O15 Mn4 Mn3 45.4(7) . .
O13 Mn4 Mn3 86.8(7) . .
O65 Mn4 Mn3 44.4(6) . .
O4W Mn4 Mn3 136.2(8) . .
O51 Mn4 Mn2 90.3(10) . .
O61 Mn4 Mn2 134.3(9) . .
O15 Mn4 Mn2 88.8(9) . .
O13 Mn4 Mn2 43.1(7) . .
O65 Mn4 Mn2 42.6(7) . .
O4W Mn4 Mn2 139.8(9) . .
Mn3 Mn4 Mn2 59.5(2) . .
O30 Mn5 O30 180.000(5) 2_775 .
O30 Mn5 O27 90.9(10) 2_775 .
O30 Mn5 O27 89.1(10) . .
O30 Mn5 O27 89.1(10) 2_775 2_775
O30 Mn5 O27 90.9(10) . 2_775
O27 Mn5 O27 180.0(15) . 2_775
O30 Mn5 O5W 93.9(11) 2_775 .
O30 Mn5 O5W 86.1(11) . .
O27 Mn5 O5W 83.4(11) . .
O27 Mn5 O5W 96.6(11) 2_775 .
O30 Mn5 O5W 86.1(11) 2_775 2_775
O30 Mn5 O5W 93.9(11) . 2_775
O27 Mn5 O5W 96.6(11) . 2_775
O27 Mn5 O5W 83.4(11) 2_775 2_775
O5W Mn5 O5W 180.0(11) . 2_775
O30 Mn5 K3 59.1(8) 2_775 2_775
O30 Mn5 K3 120.9(8) . 2_775
O27 Mn5 K3 50.1(8) . 2_775
O27 Mn5 K3 129.9(8) 2_775 2_775
O5W Mn5 K3 53.6(8) . 2_775
O5W Mn5 K3 126.4(8) 2_775 2_775
O30 Mn5 K3 120.9(8) 2_775 .
O30 Mn5 K3 59.1(8) . .
O27 Mn5 K3 129.9(8) . .
O27 Mn5 K3 50.1(8) 2_775 .
O5W Mn5 K3 126.4(8) . .
O5W Mn5 K3 53.6(8) 2_775 .
K3 Mn5 K3 180.000(1) 2_775 .
O6W K1 O29 71.3(13) 2_775 .
O6W K1 O31 68.7(12) 2_775 2_775
O29 K1 O31 85.7(14) . 2_775
O6W K1 K2 113.3(11) 2_775 .
O29 K1 K2 68.0(10) . .
O31 K1 K2 57.9(11) 2_775 .
O6W K1 W8 72.3(10) 2_775 .
O29 K1 W8 3.3(9) . .
O31 K1 W8 83.1(11) 2_775 .
K2 K1 W8 64.9(4) . .
O6W K1 W9 73.3(9) 2_775 2_775
O29 K1 W9 90.8(10) . 2_775
O31 K1 W9 6.0(9) 2_775 2_775
K2 K1 W9 57.3(3) . 2_775
W8 K1 W9 88.1(3) . 2_775
O41 K2 O34 119.7(11) 1_545 2_775
O41 K2 O26 155.7(12) 1_545 .
O34 K2 O26 83.2(8) 2_775 .
O41 K2 O3W 73.0(12) 1_545 2_775
O34 K2 O3W 93.9(11) 2_775 2_775
O26 K2 O3W 99.2(11) . 2_775
O41 K2 O31 111.5(12) 1_545 2_775
O34 K2 O31 57.1(10) 2_775 2_775
O26 K2 O31 87.1(9) . 2_775
O3W K2 O31 149.6(11) 2_775 2_775
O41 K2 O32 72.5(11) 1_545 2_775
O34 K2 O32 52.9(9) 2_775 2_775
O26 K2 O32 131.8(10) . 2_775
O3W K2 O32 102.3(11) 2_775 2_775
O31 K2 O32 54.5(9) 2_775 2_775
O41 K2 O29 130.6(11) 1_545 .
O34 K2 O29 91.8(9) 2_775 .
O26 K2 O29 49.2(8) . .
O3W K2 O29 146.9(11) 2_775 .
O31 K2 O29 52.9(9) 2_775 .
O32 K2 O29 107.0(10) 2_775 .
O41 K2 W9 107.2(10) 1_545 2_775
O34 K2 W9 32.4(7) 2_775 2_775
O26 K2 W9 96.6(7) . 2_775
O3W K2 W9 120.5(9) 2_775 2_775
O31 K2 W9 29.2(6) 2_775 2_775
O32 K2 W9 35.6(6) 2_775 2_775
O29 K2 W9 78.6(7) . 2_775
O41 K2 K1 101.4(10) 1_545 .
O34 K2 K1 92.9(9) 2_775 .
O26 K2 K1 84.1(7) . .
O3W K2 K1 172.8(9) 2_775 .
O31 K2 K1 36.4(7) 2_775 .
O32 K2 K1 79.8(8) 2_775 .
O29 K2 K1 35.2(6) . .
W9 K2 K1 65.1(4) 2_775 .
O41 K2 W8 147.8(9) 1_545 .
O34 K2 W8 89.5(7) 2_775 .
O26 K2 W8 23.8(5) . .
O3W K2 W8 121.8(9) 2_775 .
O31 K2 W8 71.2(7) 2_775 .
O32 K2 W8 124.3(8) 2_775 .
O29 K2 W8 25.6(6) . .
W9 K2 W8 90.0(3) 2_775 .
K1 K2 W8 60.8(4) . .
O41 K2 W10 106.5(9) 1_545 2_775
O34 K2 W10 23.2(7) 2_775 2_775
O26 K2 W10 92.0(6) . 2_775
O3W K2 W10 71.2(8) 2_775 2_775
O31 K2 W10 78.9(7) 2_775 2_775
O32 K2 W10 56.3(6) 2_775 2_775
O29 K2 W10 113.5(7) . 2_775
W9 K2 W10 51.2(2) 2_775 2_775
K1 K2 W10 115.3(5) . 2_775
W8 K2 W10 105.5(3) . 2_775
O41 K2 W7 143.9(11) 1_545 .
O34 K2 W7 80.4(7) 2_775 .
O26 K2 W7 23.5(5) . .
O3W K2 W7 76.2(8) 2_775 .
O31 K2 W7 104.6(7) 2_775 .
O32 K2 W7 133.2(7) 2_775 .
O29 K2 W7 72.7(6) . .
W9 K2 W7 104.4(3) 2_775 .
K1 K2 W7 107.5(4) . .
W8 K2 W7 47.24(17) . .
W10 K2 W7 80.3(3) 2_775 .
O40 K3 O27 106.9(8) . 2_775
O40 K3 O9 59.5(7) . .
O27 K3 O9 145.4(9) 2_775 .
O40 K3 O5W 60.7(8) . 2_775
O27 K3 O5W 59.6(8) 2_775 2_775
O9 K3 O5W 87.7(8) . 2_775
O40 K3 O10 103.6(9) . .
O27 K3 O10 109.4(8) 2_775 .
O9 K3 O10 52.5(7) . .
O5W K3 O10 85.3(8) 2_775 .
O40 K3 O30 118.0(9) . .
O27 K3 O30 59.3(8) 2_775 .
O9 K3 O30 97.0(8) . .
O5W K3 O30 62.0(8) 2_775 .
O10 K3 O30 50.0(7) . .
O40 K3 O37 51.3(8) . .
O27 K3 O37 89.8(8) 2_775 .
O9 K3 O37 101.1(8) . .
O5W K3 O37 88.6(8) 2_775 .
O10 K3 O37 153.0(9) . .
O30 K3 O37 144.7(8) . .
O40 K3 Mn5 97.7(6) . .
O27 K3 Mn5 34.6(6) 2_775 .
O9 K3 Mn5 111.8(7) . .
O5W K3 Mn5 37.3(6) 2_775 .
O10 K3 Mn5 79.8(5) . .
O30 K3 Mn5 34.5(5) . .
O37 K3 Mn5 110.2(6) . .
O40 K3 W10 26.3(5) . .
O27 K3 W10 96.0(7) 2_775 .
O9 K3 W10 82.2(5) . .
O5W K3 W10 71.1(6) 2_775 .
O10 K3 W10 129.8(7) . .
O30 K3 W10 133.1(7) . .
O37 K3 W10 25.3(6) . .
Mn5 K3 W10 102.5(3) . .
O40 K3 W2 83.8(6) . .
O27 K3 W2 137.5(7) 2_775 .
O9 K3 W2 25.2(5) . .
O5W K3 W2 94.7(6) 2_775 .
O10 K3 W2 29.8(5) . .
O30 K3 W2 79.1(6) . .
O37 K3 W2 125.4(6) . .
Mn5 K3 W2 104.4(4) . .
W10 K3 W2 107.4(3) . .
O40 K3 Mn2 30.9(5) . .
O27 K3 Mn2 124.2(7) 2_775 .
O9 K3 Mn2 30.5(5) . .
O5W K3 Mn2 65.4(6) 2_775 .
O10 K3 Mn2 73.6(6) . .
O30 K3 Mn2 102.4(7) . .
O37 K3 Mn2 80.0(7) . .
Mn5 K3 Mn2 99.3(3) . .
W10 K3 Mn2 56.5(2) . .
W2 K3 Mn2 53.3(2) . .
O40 K3 W7 103.3(6) . 2_775
O27 K3 W7 21.5(6) 2_775 2_775
O9 K3 W7 159.0(7) . 2_775
O5W K3 W7 72.5(6) 2_775 2_775
O10 K3 W7 130.0(6) . 2_775
O30 K3 W7 80.1(6) . 2_775
O37 K3 W7 72.2(6) . 2_775
Mn5 K3 W7 55.36(17) . 2_775
W10 K3 W7 84.8(3) . 2_775
W2 K3 W7 158.9(4) . 2_775
Mn2 K3 W7 129.5(4) . 2_775
W1 O2 W2 118.5(12) . .
W1 O3 W3 120.4(12) . .
W1 O4 W8 139.2(14) . .
W6 O5 W1 154.0(17) . .
Si1 O6 W3 124.0(16) . .
Si1 O6 W2 127.9(15) . .
W3 O6 W2 90.8(8) . .
Si1 O6 W1 122.4(13) . .
W3 O6 W1 91.4(8) . .
W2 O6 W1 89.9(9) . .
W2 O8 W3 120.7(14) . .
W2 O9 Mn2 131.0(14) . .
W2 O9 K3 112.1(12) . .
Mn2 O9 K3 105.0(9) . .
W8 O10 W2 149.2(17) . .
W8 O10 K3 106.5(11) . .
W2 O10 K3 96.9(10) . .
W4 O12 W3 145.5(15) . .
W3 O13 Mn4 128.5(15) . .
W3 O13 Mn2 131.6(16) . .
Mn4 O13 Mn2 94.4(10) . .
W4 O15 Mn4 132.1(14) . .
W4 O15 Mn3 129.5(14) . .
Mn4 O15 Mn3 92.0(10) . .
W4 O16 W5 123.7(15) . .
W6 O17 W4 122.1(15) . .
Si1 O18 W4 126.0(12) . .
Si1 O18 W5 126.8(13) . .
W4 O18 W5 91.7(9) . .
Si1 O18 W6 121.0(13) . .
W4 O18 W6 92.4(9) . .
W5 O18 W6 88.3(7) . .
W5 O19 Mn1 148.2(15) . 1_655
W6 O20 W5 119.4(13) . .
W5 O21 Mn3 132.4(14) . .
W5 O22 W7 150.4(14) . .
W6 O24 W7 141.7(15) . .
W7 O25 Mn1 176.7(19) . 2_775
W8 O26 W7 115.9(15) . .
W8 O26 K2 120.2(12) . .
W7 O26 K2 123.7(12) . .
W7 O27 Mn5 138.5(14) . .
W7 O27 K3 122.6(13) . 2_775
Mn5 O27 K3 95.3(10) . 2_775
Si1 O28 W8 130.3(16) . .
Si1 O28 W7 128.4(18) . .
W8 O28 W7 94.9(10) . .
W8 O29 K1 172.7(19) . .
W8 O29 K2 96.3(11) . .
K1 O29 K2 76.8(11) . .
W8 O30 Mn5 137.1(17) . .
W8 O30 K3 108.0(12) . .
Mn5 O30 K3 86.5(9) . .
W9 O31 K1 166.6(19) . 2_775
W9 O31 K2 92.4(13) . 2_775
K1 O31 K2 85.7(13) 2_775 2_775
W11 O32 W9 121.3(17) . .
W11 O32 K2 123.5(18) . 2_775
W9 O32 K2 85.5(10) . 2_775
W9 O33 W15 138.1(17) . .
W9 O33 W18 138.4(15) . .
W15 O33 W18 70.6(10) . .
W9 O34 W10 119.0(13) . .
W9 O34 K2 99.4(11) . 2_775
W10 O34 K2 123.9(14) . 2_775
W9 O35 Mn3 146.5(16) . .
Si2 O36 W10 126.2(16) . .
Si2 O36 W9 122(2) . .
W10 O36 W9 92.8(12) . .
Si2 O36 W11 125.1(16) . .
W10 O36 W11 90.6(13) . .
W9 O36 W11 90.5(9) . .
W10 O37 Mn1 152.2(18) . .
W10 O37 K3 97.3(13) . .
Mn1 O37 K3 105.3(11) . .
W10 O38 W12 143(2) . .
W10 O38 W23 135.8(18) . .
W12 O38 W23 64.2(10) . .
W11 O39 W10 121.7(15) . .
W10 O40 Mn2 140.9(14) . .
W10 O40 K3 109.2(12) . .
Mn2 O40 K3 105.8(9) . .
W11 O41 K2 155(2) . 1_565
W11 O42 W15 141.3(18) . .
W11 O42 W19 153.1(16) . .
W15 O42 W19 49.8(9) . .
W11 O43 W23 136.3(16) . .
W11 O43 W14 160.9(17) . .
W23 O43 W14 49.1(7) . .
W18 O44 W16 50.9(9) . .
W18 O44 Mn3 139(2) . .
W16 O44 Mn3 135.2(16) . .
W23 O45 W14 62(3) . .
W23 O45 W12 96(3) . .
W14 O45 W12 130(2) . .
W21 O46 W13 71(2) . .
W21 O46 W12 80(2) . .
W13 O46 W12 124.5(19) . .
W12 O47 W21 64.8(11) . .
W12 O47 Mn2 140.4(16) . .
W21 O47 Mn2 126.6(19) . .
Si2 O48 W23 124.6(16) . .
Si2 O48 W13 125.2(18) . .
W23 O48 W13 109.8(10) . .
Si2 O48 W21 122.9(13) . .
W23 O48 W21 98.9(12) . .
W13 O48 W21 46.3(5) . .
Si2 O48 W12 123.2(17) . .
W23 O48 W12 56.1(8) . .
W13 O48 W12 91.4(9) . .
W21 O48 W12 52.1(6) . .
Si2 O48 W14 126.8(13) . .
W23 O48 W14 39.5(5) . .
W13 O48 W14 90.2(9) . .
W21 O48 W14 110.3(10) . .
W12 O48 W14 89.3(10) . .
Si2 O48 W22 119.7(18) . .
W23 O48 W22 91.9(9) . .
W13 O48 W22 46.4(6) . .
W21 O48 W22 90.1(9) . .
W12 O48 W22 117.0(10) . .
W14 O48 W22 55.3(6) . .
W22 O50 W14 93.5(17) . .
W22 O50 W13 64.3(13) . .
W14 O50 W13 125.6(17) . .
W13 O51 W21 57.8(10) . .
W13 O51 Mn4 146.4(17) . .
W21 O51 Mn4 127.5(18) . .
W22 O52 W17 83.7(16) . .
W22 O52 W13 61.1(13) . .
W17 O52 W13 139(2) . .
W22 O52 W20 153(2) . .
W17 O52 W20 71.6(12) . .
W13 O52 W20 134.6(17) . .
W17 O54 W22 77.5(15) . .
W17 O54 W14 145.8(18) . .
W22 O54 W14 71.3(12) . .
W17 O54 W19 48.3(10) . .
W22 O54 W19 124(2) . .
W14 O54 W19 152.1(18) . .
W15 O56 W17 147(3) . .
W18 O57 W15 109(3) . .
W18 O57 W16 51.6(16) . .
W15 O57 W16 119.4(19) . .
Si2 O58 W16 127.1(16) . .
Si2 O58 W17 124.4(15) . .
W16 O58 W17 95.0(12) . .
Si2 O58 W19 133.3(18) . .
W16 O58 W19 99.5(12) . .
W17 O58 W19 41.8(6) . .
Si2 O58 W15 119.2(17) . .
W16 O58 W15 93.0(10) . .
W17 O58 W15 88.1(9) . .
W19 O58 W15 46.6(6) . .
Si2 O58 W18 122.9(15) . .
W16 O58 W18 38.1(5) . .
W17 O58 W18 112.7(13) . .
W19 O58 W18 91.0(10) . .
W15 O58 W18 61.5(6) . .
W20 O60 W17 100(3) . .
W20 O60 W16 73(2) . .
W17 O60 W16 120(2) . .
W20 O61 W16 60.8(9) . .
W20 O61 Mn4 139.7(17) . .
W16 O61 Mn4 128.0(15) . .
Si1 O64 Mn2 123.1(12) . .
Si1 O64 Mn3 120.9(13) . .
Mn2 O64 Mn3 95.7(9) . .
Si2 O65 Mn2 123.1(15) . .
Si2 O65 Mn4 123.2(14) . .
Mn2 O65 Mn4 93.9(8) . .
Si2 O65 Mn3 124.2(12) . .
Mn2 O65 Mn3 92.2(9) . .
Mn4 O65 Mn3 91.4(9) . .
Mn1 O3W K2 112.1(16) . 2_775
Mn5 O5W K3 89.0(10) . 2_775
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W1 O1 1.73(3) .
W1 O3 1.86(3) .
W1 O2 1.88(3) .
W1 O4 1.94(3) .
W1 O5 1.95(3) .
W1 O6 2.38(2) .
W2 O7 1.68(3) .
W2 O9 1.80(2) .
W2 O8 1.90(3) .
W2 O10 1.96(3) .
W2 O2 2.00(3) .
W2 O6 2.34(3) .
W2 K3 3.912(15) .
W3 O11 1.74(3) .
W3 O13 1.80(2) .
W3 O12 1.91(3) .
W3 O8 1.92(3) .
W3 O3 2.01(2) .
W3 O6 2.33(3) .
W4 O14 1.66(4) .
W4 O15 1.79(2) .
W4 O16 1.87(2) .
W4 O12 1.90(2) .
W4 O17 1.99(3) .
W4 O18 2.28(3) .
W5 O19 1.74(3) .
W5 O21 1.76(3) .
W5 O22 1.89(3) .
W5 O16 1.89(3) .
W5 O20 2.01(3) .
W5 O18 2.34(2) .
W6 O23 1.74(3) .
W6 O24 1.81(3) .
W6 O20 1.82(3) .
W6 O5 1.87(3) .
W6 O17 1.87(3) .
W6 O18 2.41(2) .
W7 O25 1.69(3) .
W7 O27 1.77(3) .
W7 O22 1.92(3) .
W7 O26 1.98(3) .
W7 O24 2.15(3) .
W7 O28 2.23(2) .
W7 K3 4.072(14) 2_775
W7 K2 4.130(15) .
W8 O29 1.72(3) .
W8 O30 1.79(3) .
W8 O10 1.85(3) .
W8 O26 1.85(2) .
W8 O4 2.15(2) .
W8 O28 2.18(3) .
W8 K1 3.814(18) .
W8 K2 3.960(14) .
W8 K3 4.087(15) .
W9 O31 1.73(3) .
W9 O35 1.75(3) .
W9 O33 1.85(3) .
W9 O34 1.92(3) .
W9 O32 2.07(3) .
W9 O36 2.30(3) .
W9 K2 3.536(16) 2_775
W9 K1 3.815(13) 2_775
W10 O37 1.63(3) .
W10 O40 1.78(2) .
W10 O38 1.90(3) .
W10 O34 1.94(3) .
W10 O39 2.00(2) .
W10 O36 2.29(4) .
W10 K3 3.790(15) .
W10 K2 4.090(14) 2_775
W11 O41 1.73(3) .
W11 O42 1.74(4) .
W11 O32 1.78(3) .
W11 O39 1.84(3) .
W11 O43 1.87(2) .
W11 O36 2.42(3) .
W12 O63 1.68(4) .
W12 O47 1.81(3) .
W12 O46 1.93(4) .
W12 O45 1.94(4) .
W12 O38 1.95(3) .
W12 O48 2.38(3) .
W13 O49 1.73(5) .
W13 O46 1.84(4) .
W13 O51 1.84(3) .
W13 O50 2.01(3) .
W13 O52 2.02(4) .
W13 O48 2.29(3) .
W14 O53 1.70(3) .
W14 O50 1.74(3) .
W14 O45 1.78(4) .
W14 O43 1.90(2) .
W14 O54 1.99(4) .
W14 O48 2.43(2) .
W15 O56 1.70(4) .
W15 O55 1.81(3) .
W15 O42 1.93(3) .
W15 O57 1.95(4) .
W15 O33 1.97(3) .
W15 O58 2.42(3) .
W16 O59 1.71(4) .
W16 O44 1.87(3) .
W16 O60 1.96(4) .
W16 O57 1.96(4) .
W16 O61 2.04(3) .
W16 O58 2.24(3) .
W17 O62 1.65(3) .
W17 O56 1.76(4) .
W17 O54 1.82(4) .
W17 O52 1.88(3) .
W17 O60 1.95(4) .
W17 O58 2.34(3) .
W18 O57 1.04(4) .
W18 O44 1.72(3) .
W18 O33 2.33(3) .
W18 O58 2.47(3) .
W19 O54 2.19(4) .
W19 O58 2.36(3) .
W19 O42 2.43(4) .
W20 O60 1.05(4) .
W20 O61 1.73(3) .
W20 O52 2.15(4) .
W21 O46 1.14(4) .
W21 O51 1.91(4) .
W21 O47 2.03(4) .
W21 O48 2.33(2) .
W22 O50 1.34(3) .
W22 O52 1.59(4) .
W22 O54 1.89(3) .
W22 O48 2.45(3) .
W23 O45 0.74(4) .
W23 O43 1.88(3) .
W23 O38 2.08(3) .
W23 O48 2.17(3) .
Si1 O6 1.60(2) .
Si1 O28 1.61(3) .
Si1 O18 1.61(3) .
Si1 O64 1.63(2) .
Si2 O65 1.62(2) .
Si2 O58 1.64(3) .
Si2 O48 1.64(3) .
Si2 O36 1.65(3) .
Mn1 O19 2.09(3) 1_455
Mn1 O25 2.15(3) 2_775
Mn1 O1W 2.19(4) .
Mn1 O3W 2.20(4) .
Mn1 O2W 2.20(3) .
Mn1 O37 2.26(3) .
Mn2 O47 2.07(3) .
Mn2 O9 2.07(3) .
Mn2 O40 2.11(3) .
Mn2 O64 2.14(2) .
Mn2 O65 2.18(3) .
Mn2 O13 2.20(3) .
Mn2 Mn3 3.174(9) .
Mn2 Mn4 3.210(10) .
Mn2 K3 3.945(16) .
Mn3 O44 2.10(3) .
Mn3 O35 2.11(3) .
Mn3 O21 2.13(3) .
Mn3 O64 2.14(3) .
Mn3 O65 2.23(2) .
Mn3 O15 2.27(3) .
Mn3 Mn4 3.182(8) .
Mn4 O51 2.06(3) .
Mn4 O61 2.10(3) .
Mn4 O15 2.15(3) .
Mn4 O13 2.17(3) .
Mn4 O65 2.22(2) .
Mn4 O4W 2.23(3) .
Mn5 O30 2.09(3) 2_775
Mn5 O30 2.09(3) .
Mn5 O27 2.10(3) .
Mn5 O27 2.10(3) 2_775
Mn5 O5W 2.23(3) .
Mn5 O5W 2.23(3) 2_775
Mn5 K3 3.683(11) 2_775
Mn5 K3 3.683(11) .
K1 O6W 1.75(3) 2_775
K1 O29 2.10(4) .
K1 O31 2.11(3) 2_775
K1 K2 3.55(3) .
K1 W9 3.815(13) 2_775
K2 O41 2.57(3) 1_545
K2 O34 2.67(3) 2_775
K2 O26 2.69(3) .
K2 O3W 2.91(4) 2_775
K2 O31 3.01(4) 2_775
K2 O32 3.04(4) 2_775
K2 O29 3.38(3) .
K2 W9 3.536(16) 2_775
K2 W10 4.090(15) 2_775
K3 O40 2.81(3) .
K3 O27 2.84(3) 2_775
K3 O9 2.86(3) .
K3 O5W 2.96(3) 2_775
K3 O10 3.16(3) .
K3 O30 3.16(3) .
K3 O37 3.22(3) .
K3 W7 4.072(14) 2_775
O19 Mn1 2.09(3) 1_655
O25 Mn1 2.15(3) 2_775
O27 K3 2.84(3) 2_775
O31 K1 2.11(3) 2_775
O31 K2 3.01(4) 2_775
O32 K2 3.04(4) 2_775
O34 K2 2.67(3) 2_775
O41 K2 2.57(3) 1_565
O3W K2 2.91(4) 2_775
O5W K3 2.96(3) 2_775
O6W K1 1.75(3) 2_775
